Ultrafast hole carrier relaxation dynamics in p-type CuO nanowires
© Othonos and Zervos; licensee Springer. 2011
Received: 10 September 2011
Accepted: 7 December 2011
Published: 7 December 2011
Ultrafast hole carrier relaxation dynamics in CuO nanowires have been investigated using transient absorption spectroscopy. Following femtosecond pulse excitation in a non-collinear pump-probe configuration, a combination of non-degenerate transmission and reflection measurements reveal initial ultrafast state filling dynamics independent of the probing photon energy. This behavior is attributed to the occupation of states by photo-generated carriers in the intrinsic hole region of the p-type CuO nanowires located near the top of the valence band. Intensity measurements indicate an upper fluence threshold of 40 μJ/cm2 where carrier relaxation is mainly governed by the hole dynamics. The fast relaxation of the photo-generated carriers was determined to follow a double exponential decay with time constants of 0.4 ps and 2.1 ps. Furthermore, time-correlated single photon counting measurements provide evidence of three exponential relaxation channels on the nanosecond timescale.
KeywordsCuO nanowires pump-probe spectroscopy carrier dynamics
Low-dimensional semiconductor nanostructures have been an active field of research due to their fascinating physical properties which are very different from their bulk counterparts. An important class of such nanostructures are semiconductor nanowires [NWs] since they may be used as building blocks for electronic and photonic devices which have attracted a great deal of attention over the past few years [1–3]. So far, a broad variety of metal-oxide [MO] NWs such as ZnO, SnO2, In2O3, and Ga2O3 have been grown and investigated in view of their potential technological applications. However, most of these MO NWs are n-type due to donors like oxygen-related defect states that reside energetically close to the conduction band edge. Moreover, p-type doping is not straightforward which limits the formation of p-n junctions and the realization of nanoscale electronic and optoelectronic devices. In contrast, cupric oxide [CuO] is a p-type semiconductor with a narrow bandgap energy (E G) reported to be between 1.3 and 1.7 eV . The p-type conductivity is attributed to the presence of negatively charged copper vacancies and interstitial oxygen . As such, CuO is regarded as an important material for applications in photovoltaic cells because of its high absorption coefficient, non-toxicity, and low cost.
Furthermore, CuO has been exploited as a heterogeneous catalyst to convert hydrocarbons into carbon dioxide and water . However, while the growth of CuO NWs has been investigated and understood in some detail [7–9], it appears that very little work has been carried out on their optical properties while nothing is known about the ultrafast carrier dynamics despite their potential to be used as building blocks in optoelectronic devices.
In this work, CuO NWs were grown on Cu via a self-catalyzed vapor-solid mechanism using dry oxidation and subsequently transferred onto quartz and Si(001) substrates for femtosecond transient absorption spectroscopy measurements, providing a detailed understanding of the ultrafast carrier relaxation dynamics in this p-type semiconductor NWs. We find a fast negative change in absorption due to the occupation of states by the photo-generated carriers mainly in the intrinsic hole region near the top of the valence band and a recovery within a few picoseconds associated with redistribution of the photo-generated carriers in nearby energy states. Intensity measurements reveal an upper fluence threshold of 40 μJ/cm2 where carrier relaxation is mainly governed by the hole dynamics. Furthermore, time-correlated single photon counting [TCSPC] photoluminescence [PL] measurements provide evidence of a three exponential relaxation dynamics on the nanosecond timescale.
CuO NWs were grown using an atmospheric pressure chemical vapor deposition reactor which consists of four mass flow controllers and a horizontal quartz tube [QT] furnace capable of reaching a maximum temperature of 1,100°C. For the growth of the CuO NWs, we used high-purity Cu sheets with a thickness of ≈0.12 mm in the form of strips having a width of ≈3 mm and length of ≈10 mm. The Cu strips were flat and straight, were cleaned sequentially in methanol, acetone, and isopropanol [IPA] under ultrasonic vibration, and then rinsed in deionized [DI] H2O; after which, they were dipped in diluted hydrochloric acid at room temperature [RT] for 20 s in order to remove any oxides. Finally, the foil was rinsed thoroughly with DI H2O and dried with N2. Several strips were loaded into a porcelain-type boat which was positioned directly above the thermocouple used to measure the heater temperature at the center of the 1"; QT. The latter was flushed using an Ar-to-O2 ratio of 500:100 sccm for 10 min, and then the temperature was ramped to the growth temperature [T G] using a slow ramp rate of 5°C/min and 100 sccm of O2. Upon reaching T G, the same flow of 100 sccm O2 was maintained for a further 1 to 4 h. The furnace was then allowed to cool down to RT using the same flow of O2. The Cu foils turned black and were removed from the 1"; QT only when the temperature was < 100°C in order to prevent cracking due to stress. The morphology of the CuO NWs were then examined with a TESCAN scanning electron microscope [SEM] (TESCAN USA, Cranberry Twp., PA, USA) while their crystal structure and phase purity were investigated using a SHIMADZU, XRD-6000, X-ray diffractometer (Shimadzu Corporation, Nakagyo-ku, Kyoto, Japan) with a Cu-Kα source, by performing a scan of θ-2θ in the range between 10° and 80°.
The dynamic behavior of carriers within the CuO NWs was investigated by measuring the temporal behavior of ultrafast time-resolved absorption obtained from simultaneous measurements of time-resolved transmission and reflection [10–12]. The experiments were carried out using a Ti/sapphire ultrafast amplifier system generating 100-fs pulses at 800 nm and running at a repetition rate of 1 kHz. A nonlinear crystal was used to generate 400 nm for the purpose of exciting the NWs, whereas part of the fundamental was used to generate a super continuum light for probing different energy states. Measurements were carried out using a typical pump-probe optical setup in a non-collinear configuration where differential reflection and transmission were utilized to determine the transient absorption.
Results and discussion
Ultrafast, time-resolved, differential absorption measurements for the CuO NWs using different probing wavelengths are shown in Figure 2. The femtosecond excitation pulse was set at 3.1 eV with the absorbed fluence estimated to be 210 μJ/cm2. At first sight, the behavior appears to be similar for all probing wavelengths; that is, there seems to be a fast decrease (pulse width limited) in optical absorption reaching a minimum, followed by a fast recovery toward a plateau within 5 to 10 ps, and then returning back to its equilibrium value over several nanoseconds.
A competing process known as 'free-carrier absorption' is also likely to occur due to secondary excitation of the photo-generated carriers by the probing photons from their initial states to higher energy states. This phenomenon will result in a positive change in the induced absorption and is observed for probing wavelengths larger than 830 nm as seen in Figure 2, where carriers undergo secondary excitation. We should point out that the temporal behavior of the recovery which is on a nanosecond timescale is the same as the one observed for the long-lived state filling, suggesting that we are probing the same states. The observed long-lived behavior in comparison with the fast recovery of the initial state filling signifies the difference of the probing states. This suggests that for the long-lived behavior, we are probably probing defects/surface states rather than valence or conduction band states.
The decay profiles of the TCSPC measurements are approximately the same for the different probing wavelengths. The decays are well described by an exponential function of the form I(t) = A1 e -t/τ 1 + A2 e -t/τ 2 + A3 exp -t/τ 3 , suggesting a complex energy level structure for the CuO NWs. The average exponential time constants and their associated strengths for the three probing wavelengths are 1.0 ns (80%), 4.8 ns (18%), and 26 ns (2%). This multi-exponential decay of the PL signal indicates the existence of non-radiative channels available to the probing carriers. Although the measured PL signal comes from a particular energy state, the non-radiative channels available to the photo-generated carriers in these states alter the population, thus making the PL decay appear multi-exponential.
In conclusion, CuO NWs have been grown by dry oxidation of high-purity Cu foils at 600°C which were harvested and transferred on quartz and Si(001) substrates. Ultrafast transient absorption measurements reveal an initial pulse width-limited negative change in the induced absorption for all probing wavelengths associated with the occupation of photo-generated carriers of intrinsic hole states in the valence band of the p-type CuO NWs. The recovery of the initial state filling for the low incident fluence (< 40 μJ/cm2) suggests two relaxation mechanisms: a fast relaxation of 0.4 ps (67%) associated with redistribution of the photo-generated carriers around the probing region and a slower relaxation mechanism of 2.1 ps (33%) corresponding to a decay channel coupled to states further from the probing region. On a longer time scale, the TCSPC measurements show decay profiles which are approximately the same for the probing wavelengths between 350 and 500 nm. The data show multi-exponential decay with time constants at 1.0 ns (80%), 4.8 ns (18%), and 26 ns (2%).
scanning electron microscope
time-correlated single photon counting.
The work in this article was partially supported by the research programs, ERYAN/0506/04 and ERYAN/0508/02, funded by the Cyprus Research Promotion Foundation in Cyprus.
- Lu W, Lieber CM: Semiconductor nanowires. J Phys D: Appl Phys 2006, 39: R387-R406. 10.1088/0022-3727/39/21/R01View ArticleGoogle Scholar
- Bachtold A, Hadley P, Nakanishi T, Dekker C: Logic circuits with carbon nanotube transistors. Science 2001, 294: 1317–1320. 10.1126/science.1065824View ArticleGoogle Scholar
- Huang Y, Duan XF, Cui Y, Lauhon LJ, Kim KH, Lieber CM: Logic gates and computation from assembled nanowire building blocks. Science 2001, 294: 1313–1317. 10.1126/science.1066192View ArticleGoogle Scholar
- Ching WY, Xu Y-N, Wong KW: Ground-state and optical properties of Cu 2 O and CuO crystals. Phys Rev B 1989, 40: 7684–7695. 10.1103/PhysRevB.40.7684View ArticleGoogle Scholar
- Musa AO, Akomolafe T, Carter MJ: Production of cuprous oxide, a solar cell material, by thermal oxidation and a study of its physical and electrical properties. Sol Energy Mater Solar Cells 1998, 51: 305–316. 10.1016/S0927-0248(97)00233-XView ArticleGoogle Scholar
- Reitz JB, Solomon EI: Propylene oxidation on copper oxide surfaces: electronic and geometric contributions to reactivity and selectivity. J Am Chem Soc 1998, 120: 11467–11478. 10.1021/ja981579sView ArticleGoogle Scholar
- Kaur M, Muthe KP, Despande SK, Choudhury S, Singh JB, Verma N, Gupta SK, Yakhmi JV: Growth and branching of CuO nanowires by thermal oxidation of copper. J Crystal Growth 2006, 289: 670–675. 10.1016/j.jcrysgro.2005.11.111View ArticleGoogle Scholar
- Jin C, Kim H, Hong C, Kim HW, Lee C: Preparation and photoluminescence properties of silica-coated CuO nanowires. App Phys A 2010, 100: 151–157. 10.1007/s00339-010-5589-0View ArticleGoogle Scholar
- Huang C-Y, Chatterjee A, Liu SB, Wu SY, Cheng C-L: Photoluminescence properties of a single tapered CuO nanowire. Appl Surf Sci 2010, 256: 3688–3692. 10.1016/j.apsusc.2010.01.007View ArticleGoogle Scholar
- Othonos A, Zervos M: Carrier relaxation dynamics in Sn x N y nanowires grown by chemical vapor deposition. J Appl Phys 2009, 106: 114303. 10.1063/1.3264721View ArticleGoogle Scholar
- Othonos A, Zervos M, Christofides C: Carrier dynamics in β-Ga 2 O 3 nanowires. JAppl Phys 2010, 108: 124302.View ArticleGoogle Scholar
- Othonos A: Probing ultrafast carrier and phonon dynamics in semiconductors. J Appl Phys 1998, 83: 1789–1830. 10.1063/1.367411View ArticleGoogle Scholar
- Li D, Hu J, Wu R, Lu JG: Conductometric chemical sensor based on individual CuO nanowires. Nanotechnology 2010, 21: 485502. 10.1088/0957-4484/21/48/485502View ArticleGoogle Scholar
- Chang S-S, Lee H-J, Park HJ: Photoluminescence properties of spark-processed CuO. Ceramics Int 2005, 31: 411415.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.